Gas sensing properties of nanocrystalline diamond at room temperature Marina Davydova*1, Pavel Kulha2, Alexandr Laposa2, Karel Hruska1, Pavel Demo1 and Alexander Kromka1
Full Research Paper Address: 1Institute of Physics, Academy of Science of the Czech Republic, Cukrovarnicka 10, 16200 Prague, Czech Republic and 2Department of Microelectronics, Faculty of Electrical Engineering, CTU in Prague, Technicka 2, 16627 Prague, Czech Republic Email: Marina Davydova* - [email protected]
Open Access Beilstein J. Nanotechnol. 2014, 5, 2339–2345. doi:10.3762/bjnano.5.243 Received: 15 August 2014 Accepted: 18 November 2014 Published: 04 December 2014 This article is part of the Thematic Series "Nanostructures for sensors, electronics, energy and environment II".
* Corresponding author Guest Editor: N. Motta Keywords: gas sensor; integrator; interdigitated electrodes; nanocrystalline diamond; response
© 2014 Davydova et al; licensee Beilstein-Institut. License and terms: see end of document.
Abstract This study describes an integrated NH3 sensor based on a hydrogenated nanocrystalline diamond (NCD)-sensitive layer coated on an interdigitated electrode structure. The gas sensing properties of the sensor structure were examined using a reducing gas (NH3) at room temperature and were found to be dependent on the electrode arrangement. A pronounced response of the sensor, which was comprised of dense electrode arrays (of 50 µm separation distance), was observed. The sensor functionality was explained by the surface transfer doping effect. Moreover, the three-dimensional model of the current density distribution of the hydrogenated NCD describes the transient flow of electrons between interdigitated electrodes and the hydrogenated NCD surface, that is, the formation of a closed current loop.
Introduction Air pollution is one of the main environmental-health related threats. Increasing amounts of noxious pollutants are emitted into the atmosphere, resulting in damage to human health and the environment. There is great interest in using sensing devices to improve the environmental and safety regulations of toxic gases in particular within buildings, underground structures, and airports.
Semiconducting solid-state gas sensors can be considered as the most promising, portable, miniaturized gas sensors because of their minimal power requirements. However, most of these sensors show poor selectivity, and the main drawbacks are slow sensor response times and recovery speeds. Even if the response time for the detection of reactive gases is rapid (e.g., within the range of seconds), in many cases, the recovery times at room
Beilstein J. Nanotechnol. 2014, 5, 2339–2345.
temperature can be from several hours up to several days. Only thermal annealing of the sensor reduces the sensor recovery speed [1,2]. Recently, much attention has been given to solid-state integrating-type (i.e., accumulating- or dosimeter-type) gas sensing devices, which are able to overcome the aforementioned drawbacks [3-7]. To date, various publications have focused on conductometric integrating gas sensors, which are able to avoid several problems of conventional gas sensors. Nevertheless, the proper choice of the sensing material plays an essential role [3,4]. Diamond is a promising sensor material and can be deposited on the existing sensor elements. Undoped diamond is an extremely good insulator and upon the formation of a covalent bond with hydrogen, exhibits semiconducting properties . This conductivity arises from free positive charge carriers (holes) in the sub-surface region and is highly sensitive to surrounding gases and/or liquids. Our previous works have shown that interdigitated electrodes (IDEs) capped with nanostructured, hydrogen-terminated, nanocrystalline diamond (NCD) were very sensitive and selective, especially towards phosgene gas [9,10]. In addition, we observed that the sensor sensitivity was strongly dependent on the total surface area. In this study, we demonstrate a gas sensor based on hydrogen (H)-terminated NCD with an integrating measurement principle. The influence of the surface area (adjusted by nucleation time) and the electrode arrangement on the sensitivity of the NCD sensor is discussed. Finally, a simulation of the distribution of the current density of H-terminated NCD is presented.
Results and Discussion Hot plasma microwave PECVD system Microwave plasma chemical vapor deposition is a well-established process for the fast growth of high quality diamond. In the present study, the hot plasma system with an ellipsoidal, cavity-like reactor was used to grow diamond films under the following conditions: sample temperature, 450 °C; power, 1 kW; gas pressure, 30 mbar; hydrogen and methane flow rates, 300 and 3 sccm (i.e., 1% dilution), respectively; and deposition time, 5 h. Figure 1a shows the SEM image of the surface morphology of the sensor substrate (Si/SiO 2 + IDEs with a separation of 200 µm) coated with the NCD layer using a 40 min nucleation time. This top view depicts the presence of an amorphous carbon shell at the diamond grains (film) and a visible development of diamond nanocrystal faceting. Moreover, the NCD primarily grew on the IDEs as was previously found . The gas-sensing properties of the hydrogenated NCD sensor with a sparse electrode arrangement of 200 µm were tested against a sequence of NH3 pulses (Figure 1b). These results demonstrated that the hydrogenated diamond sensor exhibited a clear response to each sequence of NH3, and this behavior indicated that the H-terminated NCD sensor demonstrated an integrator-type gas response. Figure 2a shows an SEM image of the surface morphology of the sensor substrate (Si/SiO 2 + IDEs with a separation of 50 µm) coated with the NCD layer after 40 min of nucleation time. The coating exhibited a continuous diamond layer with diamond grains up to 80 nm in size.
Figure 1: (a) SEM surface morphology of an NCD-coated sensor substrate with IDEs with separation of 200 µm and a nucleation time of 40 min, and (b) corresponding plot of the sensor response vs time.
Beilstein J. Nanotechnol. 2014, 5, 2339–2345.
Figure 2: (a) SEM surface morphology of an NCD-coated sensor substrate with IDEs with separation of 50 µm and a nucleation time of 40 min, and (b) corresponding plot of the sensor response vs time.
The gas-sensing properties of the hydrogenated NCD sensor with a dense electrode arrangement of 50 µm was also tested against a sequence of NH3 pulses (Figure 2b). It is evident that after being exposed to NH3 at room temperature, the sensor response is slightly higher than that of the sensor with sparse electrode arrays (i.e., 200 µm; Figure 1b). Figure 3a shows an SEM image of a sample that was nucleated for 2 min. A homogenous and continuous NCD film is observed. Figure 3b shows the plot of the sensor response as a function of time for a pulsed sequence of 100 ppm NH3. The sensor displayed a significantly more rapid sensor response compared with the previous sensor (Figure 2b) for the same NH3 exposure. Again, clear evidence of the integrator property was observed.
Overall, the hydrogenated diamond sensors exhibited a response to each sequence of NH3. These behaviors indicated that the H-terminated NCD sensors were able to accumulate NH3 gas in its water adsorbate layer, which confirms the integrator-type gas sensor property. Moreover, the NCD sensor with the most dense electrode arrangement of 50 µm and a nucleation time of 2 min (Figure 3) exhibited the highest response toward NH3 gas. A similar behavior was observed by Beer et al., wherein the resistance at room temperature decreased or increased due to the electrolytic dissociation of the gases in the H-terminated diamond layer .
Cold plasma microwave PECVD system In the following experiments, the fully-integrated sensor device on a micro-hotplate was used. In contrast to hot plasma, where
Figure 3: (a) SEM surface morphology of an NCD-coated sensor substrate with IDEs with separation of 50 µm and a nucleation time of 2 min, and (b) corresponding plot of the sensor response vs time.
Beilstein J. Nanotechnol. 2014, 5, 2339–2345.
the plasma is localized close to the substrate surface (i.e., a distance of 1–2 mm), which may cause the substrate to overheat, a linear antenna, microwave plasma, CVD system (i.e., cold plasma) was used to avoid this drawback. The main advantage of a cold plasma system is the minimization of overheating of the substrate surface due to the longer distance between the substrate and the linear antenna (i.e., 7–10 cm) . An NCD film was grown from hydrogen-rich gas mixtures of methane and carbon dioxide. A microwave pulse of 2 kW was used for each antenna side. A total gas pressure of 0.1 mbar was used and the substrate temperature was kept at 450 °C. Figure 4 shows the surface morphologies of fully-integrated sensor substrates coated with hydrogenated NCD films. Unfortunately, the SEM images also show that for the different nucleation times of 1 and 5 min, almost no differences were observed between the diamond morphologies. Both sensor substrates demonstrated a relatively smooth and continuous diamond film consisting of ultra-small grains (i.e.,